Download presentation

Published byGabriella Lawrence Modified over 3 years ago

1
**CRYSTALLOGRAPHIC POINTS, DIRECTIONS, PLANES & THE MILLER SYSTEM OF INDICES**

2
When dealing with crsytalline materials, it is often necessary to specify a particular point within a unit cell, a particular direction or a particular plane of atoms. Planes are important in crystals because if bonding is weak between a set of parallel planes, then brittle shear fracture may occur along these planes. Therefore, it is necessary to be able to specify individual crystal planes and in the case of shear to specify directions within these planes. Such identification is carried out by means of Miller Indices.

3
POINT COORDINATES The position of any point located within a unit cell is specified in terms of its coordinates as fractional multiplies of the unit cell edge lengths. To determine the point coordinates of point P, the manner in which the q, r, s coordinates of point P within the unit cell are determined. The “q” coordinate (which is a fraction) corresponds to the distance “qa” along the x-axis where “a” is the unit cell length along x-axis.

4
**CRYSTALLOGRAPHIC DIRECTIONS**

A crystallographic direction is defined as a line between to points (a vector). 1. A vector of convenient length is positioned such that it passes through the origin of the coordinate system. (Any vector can be translated throughout the crystal lattice, if parallelism is maintained). 2. The length of the vector projection on each of the three axes is determined in terms of the unit cell dimensions a, b, and c. 3. These three numbers are multiplied or divided by a common factor to reduce them to the smallest integer values. 4. The tree indices are enclosed in brackets as [uvw]. The u, v, and w integers correspond to the reduced projections along x, y, and z-axes respectively.

5
1. The vector as drawn passes through the origin of the coordinate system, and therefore no translation is necessary. 2. Projections of this vector along x, y, and z axes are a/2, b, and 0c. In terms of unit cell dimensions ½, 1, 0. 3. Reduction of these numbers to the lowest set of integers could be done through multipliying these numbers by 2 to yield 1, 2, and 0 4. The crystallographic direction is then [120]

6
**Vector A → a, a, a 1/a, 1/a, 1/a [1 1 1] Vector B → [1 1 0]**

z x y a B C A Vector A → a, a, a 1/a, 1/a, 1/a [1 1 1] Vector B → [1 1 0] Vector C → [1 1 1]

7
For some crystal structures, several nonparallel directions with different indices are actually equivalent. (The spacing of atoms along each direction is the same) For example in cubic crystals, all the directions represented by the following indices are equivalent. As a convenience, equivalent directions are grouped into a “family” which are grouped in angle brackets.

8
**Sometimes the angle between two directions may be necessary. **

A [h1 k1 l1] and B [h2 k2 l2] → the angle between them is a. A . B=|A| |B| cos a cos a = (h12+k12+l12) (h22+k22+l22) h1h2 + k1k2 + l1l2

9
**CRYSTALLOGRAPHIC PLANES**

The orientations of planes for a crystal structure are represented in a similar manner. In all but the hexagonal crystal system, crystallographic planes are specified by three Miller Indices as (hkl). Any two parallel planes are equivalent and have identical indices. The following procedure is employed in the determining the h, k, and l idex numbers of a plane:

10
1. If the plane passes through the selected origin, either another parallel plane must be constructed within the unit cell by an appropriate translation, or a new origin must be established at the corner of another unit cell. 2. At this point the crystallographic plane either intersects or parallels each of the three axes; the length of the planar intercept for each axis is determined in terms of the lattice parameters a, b, and c. 3. The reciprocals of these numbers are taken. 4. If necessary, these three numbers are changed to the set of smallest integers by multiplication or division by a common factor. 5. The integer indices are enclosed within parantheses as (hkl).

11
**1. The plane passes through the selected origin O**

1. The plane passes through the selected origin O. Therefore, a new origin must be selected at the corner of an adjacent unit cell.

12
2. The plane is parallel to the x’-axis and the intercept can be taken as ∞a. The y’ and z’ intersections are –b and c/2. Lattice parameters are ∞, -1, and 1/2. 3. Reciprocals are 0, -1, 2. 4. All are integers no reduction is necessary. 5. The crystallographic plane is (012)

15
**Example: Faces of a cubic unit cell.**

Various non-parallel planes may have similarities (crystallographically equivalent ). Such planes are referred to as “family of planes” and are designated as {h k l} Example: Faces of a cubic unit cell. (100) (010) (001) (100) (010) (001) Ξ {100}

16
PLANAR DENSITY When slip occurs under stress, it takes place on the planes on which the atoms are most densely packed. δ(hkl) = area # of atoms in a plane a2 (100) z y x Example: FCC unit cell δ(100)= 4*1/4+1 a2 = 2 a 1 r 4 4r2

17
LINEAR DENSITY When planes slip over each other, slip takes place in the direction of closest packing of atoms on the planes. The linear density of a crystal direction [h k l] is determined as: δ[h k l] = length # of atoms

18
**δ[100] = 1/a Example: [100] of cubic unit cell**

Example: Calculate planar density of the face plane (100) and linear density on the face diagonal [011] of an FCC structure. (100) a0 [011] a0

Similar presentations

OK

Solid State Physics Yuanxu Wang School of Physics and Electronics Henan University 双语教学示范课程.

Solid State Physics Yuanxu Wang School of Physics and Electronics Henan University 双语教学示范课程.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on planet jupiter Ppt on point contact diode Ppt on electricity for class 10th students Ppt on power generation by wind energy Ppt on network theory psychology 4g wireless systems seminar ppt on 4g Free download ppt on ms access 2007 Ppt on euro currency market Ppt on story of human evolution Ppt on voltage sag mitigation